#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/49/4114916.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4114916
loop_
_publ_author_name
'Xiqu Wang'
'Lumei Liu'
'Allan J. Jacobson'
_publ_contact_author_address
;
Department of Chemistry    
University of Houston,
Houston, TX 77204-5003
;
_publ_contact_author_email       ' ajjcob@uh.edu '
_publ_contact_author_fax         ' 713 743 2787 '
_publ_contact_author_name
;
Prof. Allan J. Jacobson
;
_publ_contact_author_phone       ' 713 743 2785 '
_publ_section_title
;
 Open-Framework and Microporous Vanadium Silicates
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              7812
_journal_page_last               7820
_journal_paper_doi               10.1021/ja020354l
_journal_volume                  124
_journal_year                    2002
_chemical_formula_sum            'Cs H6 Na O14 Si4 V'
_chemical_formula_weight         549.25
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           160
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_atom_sites_solution_hydrogens   IGNORED
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            9
_cell_length_a                   13.5674(19)
_cell_length_b                   13.5674(19)
_cell_length_c                   21.855(4)
_cell_measurement_temperature    293(2)
_cell_volume                     3484.0(9)
_computing_cell_refinement       SAINT
_computing_data_collection       SMART
_computing_data_reduction        SAINT
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    SHELXLTL
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.963
_diffrn_measured_fraction_theta_max 0.963
_diffrn_measurement_device_type  'SIEMENS SMART/CCD'
_diffrn_measurement_method       'NARROW FRAME, 0.3w'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0668
_diffrn_reflns_av_sigmaI/netI    0.0516
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       29
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            7021
_diffrn_reflns_theta_full        28.31
_diffrn_reflns_theta_max         28.31
_diffrn_reflns_theta_min         1.97
_exptl_absorpt_coefficient_mu    3.357
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.6105
_exptl_absorpt_correction_type   'multi-scan (SADABS)'
_exptl_crystal_colour            GREEN-BLUE
_exptl_crystal_density_diffrn    2.356
_exptl_crystal_description       PLATE
_exptl_crystal_F_000             2367
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.888
_refine_diff_density_min         -1.303
_refine_diff_density_rms         0.290
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.74(6)
_refine_ls_extinction_coef       0.0014(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.174
_refine_ls_hydrogen_treatment    NA
_refine_ls_matrix_type           full
_refine_ls_number_parameters     127
_refine_ls_number_reflns         2026
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.174
_refine_ls_R_factor_all          0.0840
_refine_ls_R_factor_gt           0.0754
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1383P)²+53.6920P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2225
_refine_ls_wR_factor_ref         0.2283
_reflns_number_gt                1755
_reflns_number_total             2026
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja020354l_07.cif
_cod_data_source_block           VSH-9CsNa
_cod_original_cell_volume        3484.0(10)
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_original_formula_sum        'H6 Cs Na O14 Si4 V'
_cod_database_code               4114916
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'-y+2/3, -x+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+1/3'
'x+2/3, x-y+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-y+1/3, -x+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+2/3'
'x+1/3, x-y+2/3, z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cs1 Cs 0.0000 0.0000 0.81102(13) 0.0433(6) Uani 1 6 d S
Cs2 Cs 0.234(3) 0.1170(16) 0.6556(9) 0.063(5) Uani 0.28(5) 2 d SP
Cs3 Cs 0.278(5) 0.139(3) 0.673(3) 0.091(11) Uani 0.28(5) 2 d SP
Cs4 Cs 0.370(3) 0.1849(14) 0.7846(9) 0.126(13) Uani 0.109(7) 2 d SP
Na Na 0.1460(3) 0.2919(7) 1.0693(3) 0.0298(16) Uani 1 2 d S
V V -0.3752(2) -0.18759(10) 0.73620(14) 0.0171(6) Uani 1 2 d S
Si1 Si -0.4422(2) -0.3289(2) 0.86724(14) 0.0124(6) Uani 1 1 d .
Si2 Si 0.2258(2) 0.2206(2) 0.93854(14) 0.0130(6) Uani 1 1 d .
O1 O 0.2438(8) 0.2251(7) 1.0101(4) 0.0298(19) Uani 1 1 d .
O2 O -0.4215(8) -0.3122(8) 0.7957(4) 0.0294(18) Uani 1 1 d .
O3 O -0.2395(12) -0.1198(6) 0.7389(7) 0.044(3) Uani 1 2 d S
O4 O -0.3356(6) -0.3230(5) 0.9067(4) 0.0151(13) Uani 1 1 d .
O5 O -0.2031(10) -0.1016(5) 0.9196(7) 0.034(3) Uani 1 2 d S
O6 O -0.4720(9) -0.2360(5) 0.8983(5) 0.023(2) Uani 1 2 d S
O7 O -0.1154(5) -0.2307(9) 0.9063(4) 0.0168(19) Uani 1 2 d S
O8 O -0.5474(4) -0.4526(4) 0.8850(4) 0.019(2) Uani 1 2 d S
OW1 O -0.6667 -0.3333 0.812(2) 0.048(4) Uiso 0.63(4) 6 d SP
OW2 O -0.6667 -0.3333 0.9993(13) 0.048(4) Uiso 1 6 d S
OW3 O 0.0000 0.0000 0.4780(13) 0.048(4) Uiso 0.99(8) 6 d SP
OW4 O 0.102(6) 0.051(3) 0.663(3) 0.048(4) Uiso 0.20(4) 2 d SP
OW5 O 0.298(3) 0.1491(17) 0.7319(19) 0.048(4) Uiso 0.39(4) 2 d SP
OW6 O -0.6667 -0.3333 0.742(3) 0.048(4) Uiso 0.37(4) 6 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Cs1 O3 98.2(3) . 3
O3 Cs1 O3 98.2(3) . 2
O3 Cs1 O3 98.2(3) 3 2
O3 Cs1 O5 130.83(15) . 3
O3 Cs1 O5 74.1(4) 3 3
O3 Cs1 O5 130.83(15) 2 3
O3 Cs1 O5 74.1(4) . .
O3 Cs1 O5 130.83(15) 3 .
O3 Cs1 O5 130.83(15) 2 .
O5 Cs1 O5 75.8(4) 3 .
O3 Cs1 O5 130.83(15) . 2
O3 Cs1 O5 130.83(15) 3 2
O3 Cs1 O5 74.1(4) 2 2
O5 Cs1 O5 75.8(4) 3 2
O5 Cs1 O5 75.8(4) . 2
O3 Cs1 O7 171.7(3) . 2
O3 Cs1 O7 87.2(2) 3 2
O3 Cs1 O7 87.2(2) 2 2
O5 Cs1 O7 44.71(10) 3 2
O5 Cs1 O7 97.6(3) . 2
O5 Cs1 O7 44.71(10) 2 2
O3 Cs1 O7 87.2(2) . .
O3 Cs1 O7 171.7(3) 3 .
O3 Cs1 O7 87.2(2) 2 .
O5 Cs1 O7 97.6(3) 3 .
O5 Cs1 O7 44.71(10) . .
O5 Cs1 O7 44.71(10) 2 .
O7 Cs1 O7 86.7(2) 2 .
O3 Cs1 O7 87.2(2) . 3
O3 Cs1 O7 87.2(2) 3 3
O3 Cs1 O7 171.7(3) 2 3
O5 Cs1 O7 44.71(10) 3 3
O5 Cs1 O7 44.71(10) . 3
O5 Cs1 O7 97.6(3) 2 3
O7 Cs1 O7 86.7(2) 2 3
O7 Cs1 O7 86.7(2) . 3
O3 Cs1 OW4 52.4(4) . 3
O3 Cs1 OW4 81.2(13) 3 3
O3 Cs1 OW4 52.4(4) 2 3
O5 Cs1 OW4 155.2(13) 3 3
O5 Cs1 OW4 122.5(9) . 3
O5 Cs1 OW4 122.5(9) 2 3
O7 Cs1 OW4 135.2(3) 2 3
O7 Cs1 OW4 107.1(13) . 3
O7 Cs1 OW4 135.2(3) 3 3
O3 Cs1 OW4 52.4(4) . 2
O3 Cs1 OW4 52.4(4) 3 2
O3 Cs1 OW4 81.2(13) 2 2
O5 Cs1 OW4 122.5(9) 3 2
O5 Cs1 OW4 122.5(9) . 2
O5 Cs1 OW4 155.2(13) 2 2
O7 Cs1 OW4 135.2(3) 2 2
O7 Cs1 OW4 135.2(3) . 2
O7 Cs1 OW4 107.1(13) 3 2
OW4 Cs1 OW4 35(2) 3 2
O3 Cs1 OW4 81.2(13) . .
O3 Cs1 OW4 52.4(4) 3 .
O3 Cs1 OW4 52.4(4) 2 .
O5 Cs1 OW4 122.5(9) 3 .
O5 Cs1 OW4 155.2(13) . .
O5 Cs1 OW4 122.5(9) 2 .
O7 Cs1 OW4 107.1(13) 2 .
O7 Cs1 OW4 135.2(3) . .
O7 Cs1 OW4 135.2(3) 3 .
OW4 Cs1 OW4 35(2) 3 .
OW4 Cs1 OW4 35(2) 2 .
Cs3 Cs2 OW4 137(4) . .
Cs3 Cs2 OW5 29(3) . .
OW4 Cs2 OW5 108(3) . .
Cs3 Cs2 O4 90(3) . 17_554
OW4 Cs2 O4 118.0(19) . 17_554
OW5 Cs2 O4 109.9(14) . 17_554
Cs3 Cs2 O4 90(3) . 15_544
OW4 Cs2 O4 117.9(19) . 15_544
OW5 Cs2 O4 109.9(14) . 15_544
O4 Cs2 O4 92.2(5) 17_554 15_544
Cs3 Cs2 O8 82(4) . 15_544
OW4 Cs2 O8 141(3) . 15_544
OW5 Cs2 O8 110.5(19) . 15_544
O4 Cs2 O8 46.8(3) 17_554 15_544
O4 Cs2 O8 46.8(3) 15_544 15_544
Cs3 Cs2 Cs4 24(3) . .
OW4 Cs2 Cs4 113(3) . .
OW5 Cs2 Cs4 5.1(14) . .
O4 Cs2 Cs4 106.5(10) 17_554 .
O4 Cs2 Cs4 106.5(9) 15_544 .
O8 Cs2 Cs4 105.4(12) 15_544 .
Cs3 Cs2 O3 90(2) . 3
OW4 Cs2 O3 62.5(15) . 3
OW5 Cs2 O3 70.6(9) . 3
O4 Cs2 O3 86.7(3) 17_554 3
O4 Cs2 O3 179.0(5) 15_544 3
O8 Cs2 O3 132.2(5) 15_544 3
Cs4 Cs2 O3 73.9(6) . 3
Cs3 Cs2 O3 90(2) . 2
OW4 Cs2 O3 62.5(15) . 2
OW5 Cs2 O3 70.6(9) . 2
O4 Cs2 O3 179.0(6) 17_554 2
O4 Cs2 O3 86.7(3) 15_544 2
O8 Cs2 O3 132.2(5) 15_544 2
Cs4 Cs2 O3 73.9(6) . 2
O3 Cs2 O3 94.3(7) 3 2
Cs3 Cs2 OW4 137(3) . 2
OW4 Cs2 OW4 17.5(10) . 2
OW5 Cs2 OW4 110.5(18) . 2
O4 Cs2 OW4 101.8(12) 17_554 2
O4 Cs2 OW4 129.2(14) 15_544 2
O8 Cs2 OW4 135.3(14) 15_544 2
Cs4 Cs2 OW4 115.3(13) . 2
O3 Cs2 OW4 51.1(11) 3 2
O3 Cs2 OW4 78.8(12) 2 2
Cs3 Cs2 OW4 137(3) . 3
OW4 Cs2 OW4 17.5(9) . 3
OW5 Cs2 OW4 110.5(18) . 3
O4 Cs2 OW4 129.2(14) 17_554 3
O4 Cs2 OW4 101.8(12) 15_544 3
O8 Cs2 OW4 135.3(15) 15_544 3
Cs4 Cs2 OW4 115.3(13) . 3
O3 Cs2 OW4 78.8(12) 3 3
O3 Cs2 OW4 51.1(11) 2 3
OW4 Cs2 OW4 34.4(17) 2 3
Cs3 Cs2 O1 74.0(7) . 15_554
OW4 Cs2 O1 103.7(6) . 15_554
OW5 Cs2 O1 77.5(6) . 15_554
O4 Cs2 O1 43.4(2) 17_554 15_554
O4 Cs2 O1 131.1(8) 15_544 15_554
O8 Cs2 O1 84.7(5) 15_544 15_554
Cs4 Cs2 O1 76.6(5) . 15_554
O3 Cs2 O1 48.0(3) 3 15_554
O3 Cs2 O1 137.6(6) 2 15_554
OW4 Cs2 O1 87.2(9) 2 15_554
OW4 Cs2 O1 121.3(11) 3 15_554
Cs2 Cs3 OW5 137(4) . .
Cs2 Cs3 OW4 31(3) . .
OW5 Cs3 OW4 106(3) . .
Cs2 Cs3 Cs4 151(3) . .
OW5 Cs3 Cs4 13(2) . .
OW4 Cs3 Cs4 120(2) . .
Cs2 Cs3 O8 87(4) . 15_544
OW5 Cs3 O8 136(4) . 15_544
OW4 Cs3 O8 118(4) . 15_544
Cs4 Cs3 O8 123(2) . 15_544
Cs2 Cs3 O4 78(3) . 17_554
OW5 Cs3 O4 128(2) . 17_554
OW4 Cs3 O4 100(3) . 17_554
Cs4 Cs3 O4 120.7(17) . 17_554
O8 Cs3 O4 46.4(4) 15_544 17_554
Cs2 Cs3 O4 78(3) . 15_544
OW5 Cs3 O4 128(2) . 15_544
OW4 Cs3 O4 100(3) . 15_544
Cs4 Cs3 O4 120.7(17) . 15_544
O8 Cs3 O4 46.4(4) 15_544 15_544
O4 Cs3 O4 89.8(9) 17_554 15_544
Cs2 Cs3 O3 79.2(19) . 3
OW5 Cs3 O3 71.6(13) . 3
OW4 Cs3 O3 59.8(12) . 3
Cs4 Cs3 O3 80.5(10) . 3
O8 Cs3 O3 131.0(9) 15_544 3
O4 Cs3 O3 84.7(6) 17_554 3
O4 Cs3 O3 157(3) 15_544 3
Cs2 Cs3 O3 79.2(19) . 2
OW5 Cs3 O3 71.6(13) . 2
OW4 Cs3 O3 59.8(12) . 2
Cs4 Cs3 O3 80.5(10) . 2
O8 Cs3 O3 131.0(9) 15_544 2
O4 Cs3 O3 157(3) 17_554 2
O4 Cs3 O3 84.7(6) 15_544 2
O3 Cs3 O3 92.1(7) 3 2
Cs2 Cs3 O1 96.2(14) . 15_554
OW5 Cs3 O1 87.6(13) . 15_554
OW4 Cs3 O1 96.9(10) . 15_554
Cs4 Cs3 O1 86.2(13) . 15_554
O8 Cs3 O1 87.2(3) 15_544 15_554
O4 Cs3 O1 44.33(18) 17_554 15_554
O4 Cs3 O1 133.3(7) 15_544 15_554
O3 Cs3 O1 48.8(3) 3 15_554
O3 Cs3 O1 140.5(5) 2 15_554
Cs2 Cs3 O1 96.2(14) . 17_544
OW5 Cs3 O1 87.6(13) . 17_544
OW4 Cs3 O1 96.9(10) . 17_544
Cs4 Cs3 O1 86.2(13) . 17_544
O8 Cs3 O1 87.2(3) 15_544 17_544
O4 Cs3 O1 133.3(7) 17_554 17_544
O4 Cs3 O1 44.32(18) 15_544 17_544
O3 Cs3 O1 140.5(5) 3 17_544
O3 Cs3 O1 48.8(3) 2 17_544
O1 Cs3 O1 166(2) 15_554 17_544
Cs2 Cs3 Si1 87(4) . 17_554
OW5 Cs3 Si1 132(3) . 17_554
OW4 Cs3 Si1 115(3) . 17_554
Cs4 Cs3 Si1 120.1(19) . 17_554
O8 Cs3 Si1 23.14(13) 15_544 17_554
O4 Cs3 Si1 24.18(18) 17_554 17_554
O4 Cs3 Si1 69.0(5) 15_544 17_554
O3 Cs3 Si1 108.6(6) 3 17_554
O3 Cs3 Si1 152.2(15) 2 17_554
O1 Cs3 Si1 64.3(2) 15_554 17_554
O1 Cs3 Si1 110.3(4) 17_544 17_554
OW5 Cs4 Cs3 12.2(19) . .
OW5 Cs4 O7 112(2) . 2
Cs3 Cs4 O7 124.6(14) . 2
OW5 Cs4 Cs2 6.6(18) . .
Cs3 Cs4 Cs2 5.6(6) . .
O7 Cs4 Cs2 118.9(11) 2 .
OW5 Cs4 OW3 136(2) . 7
Cs3 Cs4 OW3 123.4(11) . 7
O7 Cs4 OW3 112.0(9) 2 7
Cs2 Cs4 OW3 129.0(9) . 7
OW5 Cs4 O4 120.5(15) . 4
Cs3 Cs4 O4 127.9(8) . 4
O7 Cs4 O4 44.7(2) 2 4
Cs2 Cs4 O4 124.7(8) . 4
OW3 Cs4 O4 91.6(7) 7 4
OW5 Cs4 O4 120.5(15) . 2
Cs3 Cs4 O4 127.9(8) . 2
O7 Cs4 O4 44.7(2) 2 2
Cs2 Cs4 O4 124.7(8) . 2
OW3 Cs4 O4 91.6(7) 7 2
O4 Cs4 O4 81.8(4) 4 2
OW5 Cs4 O2 86.8(7) . 4
Cs3 Cs4 O2 89.2(5) . 4
O7 Cs4 O2 81.2(4) 2 4
Cs2 Cs4 O2 88.1(5) . 4
OW3 Cs4 O2 99.8(5) 7 4
O4 Cs4 O2 44.01(18) 4 4
O4 Cs4 O2 124.4(5) 2 4
OW5 Cs4 O2 86.8(7) . 2
Cs3 Cs4 O2 89.2(5) . 2
O7 Cs4 O2 81.2(4) 2 2
Cs2 Cs4 O2 88.1(5) . 2
OW3 Cs4 O2 99.8(5) 7 2
O4 Cs4 O2 124.4(5) 4 2
O4 Cs4 O2 44.01(18) 2 2
O2 Cs4 O2 157.4(9) 4 2
OW5 Cs4 Si2 115(2) . .
Cs3 Cs4 Si2 126.3(12) . .
O7 Cs4 Si2 21.74(11) 2 .
Cs2 Cs4 Si2 121.2(10) . .
OW3 Cs4 Si2 106.0(7) 7 .
O4 Cs4 Si2 23.47(16) 4 .
O4 Cs4 Si2 63.7(3) 2 .
O2 Cs4 Si2 60.9(2) 4 .
O2 Cs4 Si2 102.9(4) 2 .
OW5 Cs4 Si2 115(2) . 6
Cs3 Cs4 Si2 126.3(12) . 6
O7 Cs4 Si2 21.74(11) 2 6
Cs2 Cs4 Si2 121.2(10) . 6
OW3 Cs4 Si2 106.0(7) 7 6
O4 Cs4 Si2 63.7(3) 4 6
O4 Cs4 Si2 23.47(16) 2 6
O2 Cs4 Si2 102.9(4) 4 6
O2 Cs4 Si2 60.9(2) 2 6
Si2 Cs4 Si2 42.4(2) . 6
OW5 Cs4 Na 88.6(8) . 15_554
Cs3 Cs4 Na 83.8(4) . 15_554
O7 Cs4 Na 112.3(3) 2 15_554
Cs2 Cs4 Na 86.0(4) . 15_554
OW3 Cs4 Na 74.8(5) 7 15_554
O4 Cs4 Na 68.65(18) 4 15_554
O4 Cs4 Na 146.7(6) 2 15_554
O2 Cs4 Na 34.45(17) 4 15_554
O2 Cs4 Na 166.5(6) 2 15_554
Si2 Cs4 Na 90.61(18) . 15_554
Si2 Cs4 Na 132.3(4) 6 15_554
O1 Na O1 99.3(5) 5 .
O1 Na O2 140.7(5) 5 12
O1 Na O2 67.1(2) . 12
O1 Na O2 67.1(2) 5 8_455
O1 Na O2 140.7(5) . 8_455
O2 Na O2 99.5(5) 12 8_455
O1 Na Si2 24.7(2) 5 5
O1 Na Si2 78.5(3) . 5
O2 Na Si2 137.7(3) 12 5
O2 Na Si2 91.7(2) 8_455 5
O1 Na Si2 78.5(3) 5 .
O1 Na Si2 24.7(2) . .
O2 Na Si2 91.7(2) 12 .
O2 Na Si2 137.7(3) 8_455 .
Si2 Na Si2 55.48(14) 5 .
O1 Na Si1 137.6(3) 5 12
O1 Na Si1 92.0(2) . 12
O2 Na Si1 25.1(2) 12 12
O2 Na Si1 78.4(3) 8_455 12
Si2 Na Si1 151.1(3) 5 12
Si2 Na Si1 116.51(12) . 12
O1 Na Si1 92.0(2) 5 8_455
O1 Na Si1 137.6(3) . 8_455
O2 Na Si1 78.4(3) 12 8_455
O2 Na Si1 25.1(2) 8_455 8_455
Si2 Na Si1 116.50(12) 5 8_455
Si2 Na Si1 151.1(3) . 8_455
Si1 Na Si1 54.88(13) 12 8_455
O1 Na V 119.5(3) 5 7
O1 Na V 34.2(2) . 7
O2 Na V 33.9(2) 12 7
O2 Na V 119.4(3) 8_455 7
Si2 Na V 106.23(18) 5 7
Si2 Na V 58.25(9) . 7
Si1 Na V 58.29(9) 12 7
Si1 Na V 105.78(18) 8_455 7
O1 Na V 34.2(2) 5 8_455
O1 Na V 119.5(4) . 8_455
O2 Na V 119.4(3) 12 8_455
O2 Na V 33.9(2) 8_455 8_455
Si2 Na V 58.25(9) 5 8_455
Si2 Na V 106.23(18) . 8_455
Si1 Na V 105.78(18) 12 8_455
Si1 Na V 58.29(9) 8_455 8_455
V Na V 119.9(2) 7 8_455
O1 Na Cs4 155.4(4) 5 8
O1 Na Cs4 78.6(5) . 8
O2 Na Cs4 61.3(4) 12 8
O2 Na Cs4 128.9(5) 8_455 8
Si2 Na Cs4 135.5(3) 5 8
Si2 Na Cs4 92.2(4) . 8
Si1 Na Cs4 66.9(3) 12 8
Si1 Na Cs4 106.1(3) 8_455 8
V Na Cs4 72.0(4) 7 8
V Na Cs4 161.4(5) 8_455 8
O1 Na Cs4 78.6(5) 5 7_455
O1 Na Cs4 155.4(4) . 7_455
O2 Na Cs4 128.9(5) 12 7_455
O2 Na Cs4 61.3(4) 8_455 7_455
Si2 Na Cs4 92.2(4) 5 7_455
Si2 Na Cs4 135.5(3) . 7_455
Si1 Na Cs4 106.1(3) 12 7_455
Si1 Na Cs4 66.9(3) 8_455 7_455
V Na Cs4 161.4(5) 7 7_455
V Na Cs4 72.0(4) 8_455 7_455
Cs4 Na Cs4 93.1(9) 8 7_455
O3 V O2 104.5(5) . 6
O3 V O2 104.5(5) . .
O2 V O2 88.7(5) 6 .
O3 V O1 107.8(5) . 13_444
O2 V O1 82.0(3) 6 13_444
O2 V O1 147.6(4) . 13_444
O3 V O1 107.8(5) . 18_444
O2 V O1 147.6(4) 6 18_444
O2 V O1 82.0(3) . 18_444
O1 V O1 89.4(5) 13_444 18_444
O3 V Na 119.91(13) . 13_444
O2 V Na 42.1(3) 6 13_444
O2 V Na 118.0(3) . 13_444
O1 V Na 41.3(3) 13_444 13_444
O1 V Na 117.9(3) 18_444 13_444
O3 V Na 119.91(13) . 15_444
O2 V Na 118.0(3) 6 15_444
O2 V Na 42.1(3) . 15_444
O1 V Na 117.9(3) 13_444 15_444
O1 V Na 41.3(3) 18_444 15_444
Na V Na 120.1(2) 13_444 15_444
O3 V Cs3 49.6(6) . 2
O2 V Cs3 85.8(12) 6 2
O2 V Cs3 150.5(4) . 2
O1 V Cs3 59.9(4) 13_444 2
O1 V Cs3 116.6(11) 18_444 2
Na V Cs3 75.2(9) 13_444 2
Na V Cs3 156.1(11) 15_444 2
O3 V Cs3 49.6(6) . 3
O2 V Cs3 150.5(4) 6 3
O2 V Cs3 85.8(11) . 3
O1 V Cs3 116.6(10) 13_444 3
O1 V Cs3 59.9(4) 18_444 3
Na V Cs3 156.1(11) 13_444 3
Na V Cs3 75.2(9) 15_444 3
Cs3 V Cs3 85(2) 2 3
O3 V Cs2 45.6(5) . 2
O2 V Cs2 94.5(6) 6 2
O2 V Cs2 149.8(4) . 2
O1 V Cs2 62.3(4) 13_444 2
O1 V Cs2 109.0(5) 18_444 2
Na V Cs2 82.5(5) 13_444 2
Na V Cs2 147.5(5) 15_444 2
Cs3 V Cs2 8.8(7) 2 2
Cs3 V Cs2 76.7(15) 3 2
O3 V Cs2 45.6(5) . 3
O2 V Cs2 149.8(4) 6 3
O2 V Cs2 94.5(6) . 3
O1 V Cs2 109.0(5) 13_444 3
O1 V Cs2 62.3(4) 18_444 3
Na V Cs2 147.5(5) 13_444 3
Na V Cs2 82.5(5) 15_444 3
Cs3 V Cs2 76.7(15) 2 3
Cs3 V Cs2 8.8(7) 3 3
Cs2 V Cs2 68.3(11) 2 3
O2 Si1 O8 112.8(5) . .
O2 Si1 O6 113.0(5) . .
O8 Si1 O6 105.5(5) . .
O2 Si1 O4 114.9(4) . .
O8 Si1 O4 102.9(4) . .
O6 Si1 O4 106.9(5) . .
O2 Si1 Na 39.3(4) . 15_444
O8 Si1 Na 74.2(4) . 15_444
O6 Si1 Na 133.5(4) . 15_444
O4 Si1 Na 118.6(3) . 15_444
O2 Si1 Cs3 144.0(12) . 8_445
O8 Si1 Cs3 50.9(3) . 8_445
O6 Si1 Cs3 102.9(12) . 8_445
O4 Si1 Cs3 54.5(5) . 8_445
Na Si1 Cs3 110.5(9) 15_444 8_445
O2 Si1 Cs2 134.9(6) . 8_445
O8 Si1 Cs2 51.5(4) . 8_445
O6 Si1 Cs2 112.1(6) . 8_445
O4 Si1 Cs2 51.6(3) . 8_445
Na Si1 Cs2 103.5(4) 15_444 8_445
Cs3 Si1 Cs2 9.4(7) 8_445 8_445
O2 Si1 Cs4 59.7(4) . 3
O8 Si1 Cs4 109.1(6) . 3
O6 Si1 Cs4 144.5(6) . 3
O4 Si1 Cs4 57.8(3) . 3
Na Si1 Cs4 65.6(3) 15_444 3
Cs3 Si1 Cs4 92.9(11) 8_445 3
Cs2 Si1 Cs4 84.3(6) 8_445 3
O1 Si2 O4 110.7(4) . 4
O1 Si2 O7 112.9(4) . 2
O4 Si2 O7 106.9(5) 4 2
O1 Si2 O5 112.7(6) . 3
O4 Si2 O5 108.5(5) 4 3
O7 Si2 O5 104.8(6) 2 3
O1 Si2 Na 38.2(4) . .
O4 Si2 Na 108.3(3) 4 .
O7 Si2 Na 141.4(4) 2 .
O5 Si2 Na 78.5(5) 3 .
O1 Si2 Cs4 139.0(5) . .
O4 Si2 Cs4 63.0(4) 4 .
O7 Si2 Cs4 45.4(4) 2 .
O5 Si2 Cs4 107.3(7) 3 .
Na Si2 Cs4 170.5(4) . .
O1 Si2 Cs2 67.4(5) . 8
O4 Si2 Cs2 47.8(3) 4 8
O7 Si2 Cs2 106.7(7) 2 8
O5 Si2 Cs2 145.2(7) 3 8
Na Si2 Cs2 86.0(5) . 8
Cs4 Si2 Cs2 85.2(7) . 8
O1 Si2 Cs3 62.3(8) . 8
O4 Si2 Cs3 49.8(5) 4 8
O7 Si2 Cs3 115.4(11) 2 8
O5 Si2 Cs3 138.1(10) 3 8
Na Si2 Cs3 77.4(11) . 8
Cs4 Si2 Cs3 93.5(12) . 8
Cs2 Si2 Cs3 9.1(7) 8 8
O1 Si2 Cs1 138.0(3) . .
O4 Si2 Cs1 111.3(3) 4 .
O7 Si2 Cs1 53.8(4) 2 .
O5 Si2 Cs1 52.0(5) 3 .
Na Si2 Cs1 123.69(11) . .
Cs4 Si2 Cs1 65.0(5) . .
Cs2 Si2 Cs1 150.1(4) 8 .
Cs3 Si2 Cs1 157.8(10) 8 .
Si2 O1 V 135.3(5) . 7
Si2 O1 Na 117.1(5) . .
V O1 Na 104.5(4) 7 .
Si2 O1 Cs3 95.0(9) . 8
V O1 Cs3 91.8(4) 7 8
Na O1 Cs3 101.5(13) . 8
Si2 O1 Cs2 89.8(5) . 8
V O1 Cs2 89.7(5) 7 8
Na O1 Cs2 111.3(7) . 8
Cs3 O1 Cs2 9.9(8) 8 8
Si1 O2 V 137.0(5) . .
Si1 O2 Na 115.6(5) . 15_444
V O2 Na 104.1(4) . 15_444
Si1 O2 Cs4 98.4(5) . 3
V O2 Cs4 101.6(6) . 3
Na O2 Cs4 84.2(5) 15_444 3
V O3 Cs1 152.9(8) . .
V O3 Cs2 114.4(7) . 2
Cs1 O3 Cs2 83.7(4) . 2
V O3 Cs2 114.4(7) . 3
Cs1 O3 Cs2 83.7(4) . 3
Cs2 O3 Cs2 91.4(14) 2 3
V O3 Cs3 109.4(7) . 2
Cs1 O3 Cs3 84.4(3) . 2
Cs2 O3 Cs3 11.0(8) 2 2
Cs2 O3 Cs3 102(2) 3 2
V O3 Cs3 109.4(7) . 3
Cs1 O3 Cs3 84.4(3) . 3
Cs2 O3 Cs3 102(2) 2 3
Cs2 O3 Cs3 11.0(8) 3 3
Cs3 O3 Cs3 113(3) 2 3
Si2 O4 Si1 137.0(4) 4 .
Si2 O4 Cs2 110.4(4) 4 8_445
Si1 O4 Cs2 104.6(5) . 8_445
Si2 O4 Cs3 108.1(6) 4 8_445
Si1 O4 Cs3 101.3(5) . 8_445
Cs2 O4 Cs3 11.4(8) 8_445 8_445
Si2 O4 Cs4 93.5(5) 4 3
Si1 O4 Cs4 99.5(4) . 3
Cs2 O4 Cs4 106.9(9) 8_445 3
Cs3 O4 Cs4 118.3(15) 8_445 3
Si2 O5 Si2 147.0(10) 2 4
Si2 O5 Cs1 105.6(5) 2 .
Si2 O5 Cs1 105.6(5) 4 .
Si1 O6 Si1 124.9(7) . 6
Si2 O7 Si2 128.4(6) 3 4
Si2 O7 Cs4 112.9(4) 3 3
Si2 O7 Cs4 112.9(4) 4 3
Si2 O7 Cs1 103.6(4) 3 .
Si2 O7 Cs1 103.6(4) 4 .
Cs4 O7 Cs1 84.0(6) 3 .
Si1 O8 Si1 148.0(7) 4_445 .
Si1 O8 Cs3 105.9(3) 4_445 8_445
Si1 O8 Cs3 105.9(3) . 8_445
Si1 O8 Cs2 105.3(4) 4_445 8_445
Si1 O8 Cs2 105.3(4) . 8_445
Cs3 O8 Cs2 11.6(9) 8_445 8_445
Cs4 OW3 Cs4 117.3(3) 13_444 15_554
Cs4 OW3 Cs4 117.3(3) 13_444 14_544
Cs4 OW3 Cs4 117.3(3) 15_554 14_544
Cs2 OW4 Cs3 12.3(14) . .
Cs2 OW4 Cs1 117(3) . .
Cs3 OW4 Cs1 104(3) . .
Cs2 OW4 Cs2 136.3(11) . 3
Cs3 OW4 Cs2 137.3(9) . 3
Cs1 OW4 Cs2 77.9(14) . 3
Cs2 OW4 Cs2 136.3(11) . 2
Cs3 OW4 Cs2 137.2(9) . 2
Cs1 OW4 Cs2 77.9(14) . 2
Cs2 OW4 Cs2 85.4(17) 3 2
Cs3 OW5 Cs4 154(4) . .
Cs3 OW5 Cs2 13.9(18) . .
Cs4 OW5 Cs2 168(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cs1 O3 3.225(16) .
Cs1 O3 3.225(16) 3
Cs1 O3 3.225(16) 2
Cs1 O5 3.365(14) 3
Cs1 O5 3.365(14) .
Cs1 O5 3.365(14) 2
Cs1 O7 3.418(10) 2
Cs1 O7 3.418(10) .
Cs1 O7 3.418(10) 3
Cs1 OW4 3.44(7) 3
Cs1 OW4 3.44(7) 2
Cs1 OW4 3.44(7) .
Cs2 Cs3 0.65(5) .
Cs2 OW4 1.56(8) .
Cs2 OW5 1.83(5) .
Cs2 O4 3.214(14) 17_554
Cs2 O4 3.214(14) 15_544
Cs2 O8 3.22(2) 15_544
Cs2 Cs4 3.24(4) .
Cs2 O3 3.325(16) 3
Cs2 O3 3.325(16) 2
Cs2 OW4 3.51(7) 2
Cs2 OW4 3.51(7) 3
Cs2 O1 3.754(15) 15_554
Cs3 OW5 1.30(8) .
Cs3 OW4 2.08(10) .
Cs3 Cs4 2.66(8) .
Cs3 O8 3.19(2) 15_544
Cs3 O4 3.28(3) 17_554
Cs3 O4 3.28(3) 15_544
Cs3 O3 3.385(16) 3
Cs3 O3 3.385(16) 2
Cs3 O1 3.629(13) 15_554
Cs3 O1 3.629(13) 17_544
Cs3 Si1 3.95(2) 17_554
Cs4 OW5 1.42(5) .
Cs4 O7 3.12(2) 2
Cs4 OW3 3.54(3) 7
Cs4 O4 3.607(15) 4
Cs4 O4 3.607(15) 2
Cs4 O2 3.671(10) 4
Cs4 O2 3.671(10) 2
Cs4 Si2 4.040(18) .
Cs4 Si2 4.040(18) 6
Cs4 Na 4.163(11) 15_554
Na O1 2.336(10) 5
Na O1 2.336(10) .
Na O2 2.367(10) 12
Na O2 2.367(10) 8_455
Na Si2 3.365(6) 5
Na Si2 3.365(6) .
Na Si1 3.370(6) 12
Na Si1 3.370(6) 8_455
Na V 3.427(4) 7
Na V 3.427(4) 8_455
Na Cs4 4.163(11) 8
Na Cs4 4.163(11) 7_455
V O3 1.595(15) .
V O2 1.970(9) 6
V O2 1.970(9) .
V O1 1.990(8) 13_444
V O1 1.990(8) 18_444
V Na 3.427(4) 13_444
V Na 3.427(4) 15_444
V Cs3 4.194(8) 2
V Cs3 4.194(7) 3
V Cs2 4.239(8) 2
V Cs2 4.239(7) 3
Si1 O2 1.585(8) .
Si1 O8 1.615(4) .
Si1 O6 1.650(6) .
Si1 O4 1.651(7) .
Si1 Na 3.370(6) 15_444
Si1 Cs3 3.95(2) 8_445
Si1 Cs2 3.967(19) 8_445
Si1 Cs4 4.206(8) 3
Si2 O1 1.580(8) .
Si2 O4 1.612(7) 4
Si2 O7 1.624(5) 2
Si2 O5 1.633(5) 3
Si2 Cs2 4.068(9) 8
Si2 Cs3 4.083(14) 8
O1 V 1.990(8) 7
O1 Cs3 3.629(13) 8
O1 Cs2 3.754(15) 8
O2 Na 2.367(10) 15_444
O2 Cs4 3.671(10) 3
O3 Cs2 3.325(16) 2
O3 Cs2 3.325(16) 3
O3 Cs3 3.385(16) 2
O3 Cs3 3.385(16) 3
O4 Si2 1.612(7) 4
O4 Cs2 3.214(15) 8_445
O4 Cs3 3.28(3) 8_445
O4 Cs4 3.607(15) 3
O5 Si2 1.633(5) 2
O5 Si2 1.633(5) 4
O6 Si1 1.650(6) 6
O7 Si2 1.624(5) 3
O7 Si2 1.624(5) 4
O7 Cs4 3.12(2) 3
O8 Si1 1.615(4) 4_445
O8 Cs3 3.19(2) 8_445
O8 Cs2 3.22(2) 8_445
OW1 OW6 1.52(9) .
OW3 Cs4 3.54(3) 13_444
OW3 Cs4 3.54(3) 15_554
OW3 Cs4 3.54(3) 14_544
OW4 Cs2 3.51(7) 3
OW4 Cs2 3.51(7) 2
